The Ag deposition on TiO2 nanoparticles (Ag-TiO2 NPs) and N-TiO2 nanoparticles (Ag-N-TiO2 NPs) has been made by electrochemical methodology in view of improved antibacterial properties and enhanced photocatalytic activity under visible light irradiation. The particle size in powder and in dispersion showed similar values and good stability in aqueous medium which made them suitable for use in leather surface covering for new multifunctional properties development. The diffuse reflectance spectra of Ag-TiO2 NPs, Ag-N-TiO2 NPs and TiO2 NPs have been investigated and correlated with their photocatalytic performances under UV and visible light against different silver concentrations. The leather surfaces treated with Ag-N-TiO2 NPs showed advanced self-cleaning properties under visible light exposure through the hydrophilic mechanism of organic soil decomposition. Moreover the bacterial sensitivity and proven fungitoxic properties of Ag-N-TiO2 NPs leads to the possibility of designing new multifunctional additives to extend the advanced applications for more durable and useable materials.
One of the challenges of large scale application of titanium dioxide nanoparticles is the increased spectral photosensitivity to the visible light domain which can be reached by doping or surface deposition of photocatalysts with metals and/or non-metals. The preparation method for doped photocatalysts is essential for the catalyst’s activity performance under visible light [1, 2].
The enhanced self-cleaning or antimicrobial properties of silver doped or deposited titanium dioxide (TiO2) nanocomposites were shown in different studies in which they were synthesized by physical [3–9] or chemical techniques [10–13].
The improved photocatalytic activity of silver-titanium dioxide nanocomposites (Ag-TiO2 NP) is explained by the role of silver as an electron trap that inhibits the recombination of electron-hole pairs generated by light on the TiO2 surface [14–19]. The concentration of silver nanoparticles (Ag NP) was also found to be important for extending the light absorption of nano titanium dioxide in the visible light domain, an effect of electron traps in TiO2 band gap .
Antibacterial activity against Escherichia coli under visible light was revealed for 0.15% silver doped titanium dioxide while a concentration of 0.05% dopant exhibited the highest decomposition efficiency of Rhodamine B . Improved properties against bacteria and Rhodamine B were also registered for a filtration membrane treated with silver doped titanium dioxide . Ag/TiO2 nanofibers prepared by combining electrospinning technology and the solvothermal route also showed excellent properties for Rhodamine B photo-decomposition .
Recently, the heterogeneous catalyst based on silver and copper nanoparticles, deposited by dipping on cotton fabric showed excellent self-cleaning properties against organic matters. This marked the beginning of the era of multifunctional consumer goods treated with photocatalysts, active in visible light [4, 24]. The antimicrobial properties of textiles can be induced by a large number of inorganic based nanoparticles which require facile manufacturing techniques for scale-up at industrial level .
Silver nanoparticles proved to be effective across a wide antibacterial spectrum both in solution and in different nanocomposites for applications to medical products [26, 27]. Silver nanoparticles’ antibacterial mechanism was demonstrated through the release of a low concentration of silver ions  which were able to generate reactive oxygen species resulting in oxidative damage to bacteria cells . In other studies, the excellent antimicrobial properties of Ag-TiO2 nanocomposites  and films  were attributed to the synergistic generation of zero valent nanosilver [31, 32].
Our research should be viewed in light of the development of materials with multifunctional properties and the reduction of volatile organic compounds used as biocidal or dry cleaning chemicals. This paper presents new photocatalysts based on Ag-TiO2 and Ag-N-TiO2 nanoparticles synthesized by via the electrochemical route and their application to leather surface coating. The electrochemical synthesis method is recognized as a versatile low temperature approach which is easy to scale up. This synthesis method allows the control of the final product characteristics by varying parameters such as potential, current density, temperature and pH .
TiO2 and N-TiO2 nanopowders of 99.5% purity were supplied by TitanPE Technologies, Inc., China (surface area of 115 m2/g and average pore size of 130 Ǻ).
Sodium polyacrylate (Na-PAA) with average Mw of 2100, Orange II (OII), Methylene blue (MB) dyes were of analytical grade and supplied by Sigma-Aldrich Chemie GmbH, Germany. The deionized water used had a resistivity of 18μΩ cm and a pH value of 5–7.
Sheepskin leathers were manufactured in the Leather Research Department’s pilot plant according to the ecological technologies available on the market.
2.2 Synthesis of doped titania nanoparticles
The method of obtaining Ag-TiO2 and Ag-N-TiO2 composite nanopowders consisted of in situ electrochemical synthesis of Ag nanoparticles in a disperse aqueous suspension of TiO2 NPs or N-TiO2 NPs in the presence of Na-PAA using deionized water whilst stirring vigorously. The electrochemical method used is also known as “sacrificial anode method” which results in anodic solubilisation of Ag electrodes in aqueous medium [34, 35]. The electrochemical synthesis setup consisted of a cell with two Ag electrodes of 99.999% purity. The electrode plates (155x27x0.5 mm) were connected to a constant current generator in the range of 1-5 mA. Current densities between 0.01-0.06 mA.cm-2 were applied for 5 h by a constant current pulse reversed generator with a mechanical stirrer. Work parameters were: 10g/L TiO2 NPs or N-TiO2 NPs dispersions, 1g/L Na-PAA, at 20 °C and shaking speed of 500 rotations/min. Ag-TiO2 NPs and Ag-N-TiO2 NPs dispersions were centrifuged and the separated slurries were dried in oven. The obtained powders were milled and finely ground by using a Specamill grinding mixer. Nanocomposites of Ag-TiO2 NPs and Ag-N-TiO2 NPs with 0.53%-1.3% Ag concentrations were synthesized via the electrochemical method. After the characterization, the selected nanopowders were used for leather surface finishing (Figure 1).
2.3 Chemical-physical characterizations of Ag-TiO2 NPs and Ag-N-TiO2 NPs
Chemical-physical characterizations of Ag-TiO2 NPs and Ag-N-TiO2 NPs were performed for silver concentration by Inductively Coupled Plasma - Optical Emission Spectrometry (ICP–OES, Agilent 725) according to ASTM E 1479-99(2011) standard. Powder morphology and surface composition analysis were determined by Scanning Electron Microscopy coupled with Energy Dispersive X-Ray spectroscopy (SEM, EDX, Quanta 250 GEI). Measurement of particle size in powder form were performed by Transmission Electron Microscopy (TEM, Philips EM 410). Particle size and Zeta potential evaluation in water dispersion of 0.1% NPs were measured by Dynamic Light Scattering (DLS, Zetasizer Nano ZS, Malvern). UV-Vis diffuse reflectance spectra measurements (JASCO V 570 spectrophotometer, equipped with integrating sphere) and photocatalytic activity of Ag-TiO2 NPs, Ag-N-TiO2 NPs and TiO2 NPs in dispersion were tested on OII solution after exposure to UV and Vis light and by UV-Vis spectra recording at λ = 365 nm.
2.4 Leather surface finishing with Ag-TiO2 NPs, Ag-N-TiO2 NPs and TiO2 NPs and characterisation
The selected Ag-TiO2 and Ag-N-TiO2 nanopowders were embedded in finishing layers based on film forming polymers. This followed classical technologies based on spraying the aqueous composites on leather surface [36, 37].
The leather surface was investigated for finishing film morphology characterization and Ag identification using SEM/EDX (Quanta 200 FEI). Self-cleaning properties under UV (VL 204 lamp with irradiation at 365 nm) and Vis light (500W halogen lamp with irradiation between 400-700 nm) exposure of simulated stains (ball pen ink, OII, MB dyes) were recorded by photography. The antimicrobial sensitivity and resistance against Epidermophyton floccosum, Escherichia coli ATCC 25922, Staphylococcus aureus ATCC 25923, Candida albicans ATCC 26790, Candida albicans 1726 and Candida albicans 1760 strains were tested according to EN ISO 20645 and ISO 20743. The dynamic contact angle modification for water drop on leather surface was measured using a contact angle analyzer (VGA Optima XE).
3 Results and Discussion
The powder morphology showed that the grains of Ag-N-TiO2 and Ag-TiO2 nanopowders were round, with uniform shape and size under 30 nm. The doping Ag was identified by EDX analysis proving a successful loading of silver on the surface of TiO2 NPs and N-TiO2 NPs (Figure 2).
TEM analyses of Ag-N-TiO2 and Ag-TiO2 nanopowders showed higher particle sizes as compared to N-TiO2 and TiO2 nanopowders indicating that electrochemical deposition occurred on the particle surface. According to literature, the inclusion of silver nanoparticles inside titania crystallite would decrease the particle sizes of nanocomposites . In Figure 3 are presented the TEM images for TiO2 NPs with particle size of 25 nm, N-TiO2 NPs with 28 nm, Ag-TiO2 NPs with 31 nm and Ag-N-TiO2 NPs with 40 nm.
As the nanopowders are used in leather finishing aqueous composites, the particle size and the Zeta potential were measured for Ag-TiO2 NPs and Ag-N-TiO2 NPs by DLS. In Figures 4a and 4c it can be seen that the average particle sizes of Ag-TiO2 NPs and Ag-N-TiO2 NPs are 50 nm and of 55 nm respectively, similar values to those measured by TEM. It is known that Zeta potential below -25 mV and above +25 mV indicates a stable nanoparticles surface without aggregation tendency. Lower values of Zeta potential suggest aggregation of nanoparticles due to Van der Waals forces. In Figures 4b and 4d, Zeta potential values of -41.4 mV and – 47.4 mV for Ag-TiO2 NPs and Ag-N-TiO2 NPs can be seen, corresponding to stable water dispersions. The stability of NP dispersions represents an important characteristic for uniform distribution on leather surface and surface contact increase.
UV-Vis diffuse reflectance spectra (DRS) of Ag-TiO2 NPs, Ag-N-TiO2 NPs and TiO2 NPs showed an increase of photocatalytic activity in the visible range. This is due to the influence of silver and especially of silver and nitrogen elements which shift the absorbance from the UV to visible domain in accordance with date from the literature . As can be seen in Figure 5, 0.5% Ag and N enhance the absorbance value and generate the shifting of the so-called tail band to the visible domain as compared to other concentrations of Ag and with TiO2 NPs. It can be estimated that the photocatalytic activity is increased due to electron acceptor role of Ag and the facilitation of more holes to be transported at the surface. The results suggest that the Ag concentrations of 1.3% and 0.8% blocked the light from the TiO2 NPs surface with the decrease in photo-induced electrons-holes and catalytic efficiency, in accordance with literature [39, 40].
The photocatalytic activities of Ag-TiO2 NPs and Ag-N-TiO2 NPs were tested on solutions of 20 ppm OII with 0.5 g/L nanopowder exposed to UV and visible light. The photocatalytic activity under UV light was evaluated depending on Ag concentration with the aim of selecting the most efficient nanocomposite. Figure 6 shows the improved efficiency of OII dye photocatalytic decomposition recorded at λ = 365 nm after 60 minutes of UV exposure under the influence of doped TiO2 NPs. The concentration of 0.5% Ag deposited on TiO2 NPs surface was shown to be more effective as compared to 1.3% and 0.8% Ag concentrations, in agreement with DRS spectra (Figure 5) and literature data . Ag electrochemically deposited on N-TiO2 NPs improves the photocatalytic efficiency of OII decomposition under UV light.
The photocatalytic activity of Ag-TiO2 NPs, Ag-N-TiO2 NPs and TiO2 NPs under visible light was measured after 30 minutes of exposure to visible light (Figure 7) and showed the best photocatalytic decomposition of 20 ppm OII dye in solution in the presence of 0.5g/L Ag-N-TiO2 NPs.
The selected NPs for leather surface finishing were Ag-TiO2 NPs and Ag-N-TiO2 NPs with 0.5% Ag concentration. The morphology of leather surfaces and the identification of silver were performed using SEM/EDX analyses and are presented in Figure 8. The images showed a uniform distribution of NPs clusters and concentrations of 0.2% Wt Ag to 0.6% Wt Ag on the leather surface.
The self-cleaning properties of leather surface treated with Ag doped TiO2 NPs were tested after the simulation of model staining with ball pen ink, MB and OII dyes and by monitoring the organic stain degradation over time under exposure to UV and visible light.
In Figure 9 are presented the photos of organic stains degradation after 70 hours of exposure to visible light and 100 hours of exposure to UV light. The ball pen ink, MB and OII stains were degraded only after the visible light exposure of the leather surface treated with Ag-N-TiO2 NPs. The improved self-cleaning effects on leather surface were recorded in the case of treatments with Ag-TiO2 NPs and mostly with Ag-N-TiO2 NPs under visible light exposure, thus enhancing the leather durability and consumer comfort. The results are consistent with information in the literature regarding the photocatalytic enhancement of Ag-N-TiO2 NPs under visible light exposure against methyl orange dye or methylene blue decomposition. This was explained by the decrease in rate of electron–hole pair recombination on TiO2 NPs surface [41, 42] and increased surface area . The Fermi levels of silver and nitrogen are lower than those of TiO2, and photoexcited electrons can be transferred from the conduction band to the dopant particles deposited on the surface of TiO2, while photogenerated valence band holes remain in the TiO2. These activities greatly reduce the possibility of electron-hole recombination, resulting in efficient separation and stronger photocatalytic reactions [44, 45]. The mechanism of improved visible light activity (VLA) of TiO2 NPs doped with noble metal nanoparticles is attributed to the promotion of interfacial charge separation by electron attraction and increase of lifetime of the charge separated species .
The results showed clearly that the enhanced photocatalytic activity of Ag-N-TiO2 NPs against organic matters was successfully transferred not only in aqueous dispersion but also to leather surface treated with film forming polymers which are innovative approaches as compared to the literature [36, 47].
The possibility to avoid solvent use for dry cleaning and restoring of leather items is an important ecological issue of NPs use in leather surface finishing. Moreover in the last decades the demand for light colors, the most sensitive to soiling, have increased .
The photocatalytic activity of NPs on leather surface in the presence of H2O leads to a modification of the contact angle due to the generation of hydroxyl radicals (•OH) and superoxide anions (•O2-) after exposure to UV and visible light. The modification of the contact angle of a water drop under the treated leather surface was evaluated over time after exposure to UV and visible light. The hydrophilicity increased whilethecontact angle decreased under light exposure of leather surface treated with Ag-N-TiO2 NPs, Ag-Tia2 NPsandTi02NPt. After 2 hours of iisnCiatsen thecoctaet angle drops for leather surfacetreated with Ag-N-TiO2 NPs from 65°-75° to 7°. Ag and N elements act synergistically to mcreere Ti02 NPs photoreactivity and surface hydrophilicity. The leather surfaces treated with Ag-TiO2 NPs and Ag-N-TiO2 NPs showed the highest hydrophilicity aft er exposure to UV and visible light as compared to TiO2 NPs, proving that the self-cleaning eff ects are generated through photoinduced catalytic eff ectsIn Figure 10 it can be seen that the induced hydrophilicity aft er exposure to visible light is signifi cantly improved due to the Ag and N elements deposited on TiO2 NP surface, in accordance with the performances of self-cleaning test results.
The use of silver based NPs as biocides is well-known for The use of silver based NPs as biocides is well-known for treatment of textiles, plastics and other materials for medical [49-51] or every day use. Leather with antimicrobial properties is very important for footwear lining in the case of diabetic patients or in everyday use, taking into consideration the high rate of reported foot mycosis .The other area of application is upholstery leathers with antimicrobial resistance for the furniture or automotive industries.
The leather surface sensitivity at direct contact with Escherichia coli ATCC 25922 and Staphylococcus aureus ATCC 25923 was eveluated according to EN ISO 20645 for leather surface treated with Ag-N-TiO2 NPs and Ag-TiO2 NPs in comparison to untreated leather surfaces. In Figure 11 there are the optical microscopy images (10X) of colonies from the areas contacted with leather surface (B) and from the media in adjacent areas (A). It can be seen that the treated leather surfaces (Figure 11 a, b, d, e, B areas)are sensitive to tested bacteria as compared to untreated leather surfaces (Figure 11 c, f B areas). A clearer medium after the contact with Ag-TiO2 NPs treated leather surfaces (Figure 11 a and d) can be seen as compared to the medium aft er contact with leather surface treated with Ag-TiO2 NPs (Figure 11 b and e), in correlation to the test results for fungus resistance (Table 1).
|Fungus strain||T0CFU/mlAg-N-TiO2NPs||T24 CFU/ml||Reduction%||T0CFU/mlAg-TiO2 NPs||T24CFU/ml||Reduction%|
|Candida albicans ATCC 26790||6.6×103||0||100||6.6×103||6.6×103||0|
|Candida albicans 1726||173×103||13.3×103||92.3||173×103||46.6×103||73|
|Candida albicans 1760||56×103||0||100||56×103||20×103||64.3|
The fungistatic activity of leather surfaces treated with Ag-N-TiO2 NPs and Ag-TiO2 NPs was evaluated according to ISO 20743 using the absorption method by direct inoculation of fungi (Epidermophyton fl occosum, Candida albicans ATCC 26790, Candida albicans 1726 and Candida albicans 1760) on leather surface and quantifi cation of viable colonies aft er 24 hours. The results are presented in Table 1 and show that leather surface treated with Ag-N-TiO2 NPs has excellent resistance against Candida albicans ATCC 26790, Candida albicans 1760 and good resistance against Epidermophyton floccosum, specific fungus for footwear interior.
Ultrastructural analyses elucidating the interaction between Ag NPs with Candida spp have not been reported. In 2014, TEM analysis achieved by Vazquez-Muñoz et al., revealed a high accumulation of Ag NPs outside the cells but also smaller nanoparticles localized throughout the cytoplasm . These results suggest that the mode of action of Ag NPs is to aggregate outside the fungal cells, releasing silver ions and thus inducing cell death through the reduction process resulting from the interaction of cell components with ionic silver. As the Ag NPs’ mechanisms of action are not clear yet, is difficult to explain the comportment of the different C. albicans strains. Both strains, Candida albicans 1726 and Candida albicans 1760, are clinical isolates that probably become more sensitive to different antimicrobial substances in vitro. The behavior of the C. albicans ATCC 26790 strain with respect to the interaction with Ag NPs is unknown, therefore further investigation is necessary to elucidate this effect.
The improved behavior of leather surfaces treated with Ag-N-TiO2 NPs is attributed to the higher hydrophilic surfaces favorable for the contact of NPs with bacteria and fungus. The results suggest that the increased surface contact [54, 55] and the generation of reactive oxygen species on leather surface treated with electrochemically nano Ag deposited on N-TiO2 NPs can explain the antimicrobial effectiveness. The improved resistance of Ag-N-TiO2 NPs against bacteria strains was also confirmed by other studies [56, 57]. In our work the resistance against bacteria and fungus strains of Ag-N-TiO2 NPs was successfully transferred on leather surface coating.
Silver nanoparticles were deposited on TiO2 NPs and N-TiO2 NPs by electrochemical method and showed advanced photoinduced catalytic properties in the visible domain. The particle size increased by silver deposition from 20 nm and 25 nm for TiO2 NPs and N-TiO2 NPs to 31 nm and 40 nm for Ag-TiO2 NPs and Ag-N-TiO2 NPs according to transmission electron microscopy analyses. The water dispersions of Ag-TiO2 NPs and Ag-N-TiO2 NPs were stable with Zeta potential of −41.4 mV to –47.4 mV. Diffuse reflectance spectra of Ag-TiO2 NPs and Ag-N-TiO2 NPs shifted to the visible domain as compared to TiO2 NPs. Photocatalytic properties of silver deposited on TiO2 NPs and N-TiO2 NPs tested on Orange II dye solution under UV and visible light exposure were investigated for different silver concentrations and resulted in the selection of the 0.5% concentration as the most efficient in visible light. The enhanced photocatalytic properties in the visible light domain were confirmed under leather surface through self-cleaning stains of ball pen ink, Orange II and methylene blue dyes that were recorded for treated leather surfaces with Ag-N-TiO2 NPs. The antimicrobial resistance of leather surface treated with Ag-N-TiO2 NPs was excellent against Candida albicans ATCC 26790, Candida albicans 1760 and good against Epidermophyton floccosum. The leather surface sensitivity tests at direct contact with Escherichia coli ATCC 25922 and Staphylococcus aureus ATCC 25923 proved to be resistant for both treatments based on Ag-TiO2 and Ag-N-TiO2 nanoparticles. The improved antimicrobial sensitivity and resistance as well as the self-cleaning effects under visible light were attributed to the photocatalytic induced hydrophilic properties on leather surface treated with silver electrochemically deposited on N-TiO2 NPs.
The leather surface covered with Ag-N-TiO2 NPs showed enhanced self-cleaning and antimicrobial properties, increasing the leather durability and usability and paving the way for designing new nanoparticles with multifunctional functionalities.
This work was supported in part by a grant of the Romanian National Authority for Scientific Research and Innovation, CCCDI – UEFISCDI, project number 15, NANO_SAFE_LEATHER, under the frame of SIINN, the ERA-NET for a Safe Implementation of Innovative Nanoscience and Nanotechnology and project number 167, Selfpropiel.
 Banerjee S., Pillai S. C., Falaras P., O’Shea K. E., Byrne J. A., and Dionysiou D. D., New Insights into the Mechanism of Visible Light Photocatalysis, J. Phys. Chem. Lett., 2014, 5, 15, 2543–2554.10.1021/jz501030xSearch in Google Scholar PubMed
 Pengfei J., Masato T., Cuong T.-M. and all., Recent advances in visible light-responsive titanium oxide-based photocatalysts, Research on Chemical Intermediates, 2010, 36, 4, 327–347.10.1007/s11164-010-0142-5Search in Google Scholar
 Yufei W., Yan L., He X., Li J., Wang D., Controlled fabrication of Ag/TiO2 nanofibers with enhanced stability of photocatalytic activity, J. Mater Sci El, 2016, 27, 5, 5190–5196.10.1007/s10854-016-4412-xSearch in Google Scholar
 Xu L., Zhang D., Ming L., Jiao Y., and Chen F., Synergistic effect of interfacial lattice Ag+ and Ag0 clusters in enhancing the photocatalytic performance of TiO2 Phys. Chem. Chem. Phys., 2014, 16, 19358–19364.10.1039/C4CP02658FSearch in Google Scholar
 Li M., Noriega-Trevino M.E., Nino-Martinez N., Marambio-Jones C., Wang J., Damoiseaux R., Ruiz F., and Hoek E. M. V., Synergistic Bactericidal Activity of Ag-TiO2 Nanoparticles in Both Light and Dark Conditions, Environ. Sci. Technol., 2011, 45, 20, 8989–8995.10.1021/es201675mSearch in Google Scholar PubMed
 Zhang H., Liang C., Liu J., Tian Z., Wang G., and Cai W., Defect-Mediated Formation of Ag Cluster-Doped TiO2 Nanoparticles for Efficient Photodegradation of Pentachlorophenol, Langmuir, 2012, 28, 8, 3938–3944.10.1021/la2043526Search in Google Scholar PubMed
 Albiter E., Hai Z., Alfaro S., Remita H., Valenzuela M. A., Colbeau-Justin C., A Comparative Study of Photo-Assisted Deposition of Silver Nanoparticles on TiO2 J Nanosci Nanotechnol, 2013, 13, 7, 4943–4948.10.1166/jnn.2013.7590Search in Google Scholar PubMed
 Hyunyoung K., Kwangmin L., Photocatalytic Activity of TiO2 Nanotubes Doped with Ag Nanoparticles, J Nanosci Nanotechnol, 2013, 13, 8, 5597–5600.10.1166/jnn.2013.7035Search in Google Scholar PubMed
 Sobana N., Muruganadham M., Swaminathan M., Nano-Ag particles doped TiO2 for efficient photodegradation of direct azo dyes, J. Mol. Catal. A: Chem., 2006, 258, 124–132.10.1016/j.molcata.2006.05.013Search in Google Scholar
 Zou X., Silva R., Huang X., Jafar F., Al-Sharab J. and Asefa T., A Self-Cleaning Porous TiO2-Ag Core-Shell Nanocomposite Material for Surface-Enhanced Raman Scattering, Chem. Commun., 2013, 49, 382–384.10.1039/C2CC35917KSearch in Google Scholar
 Behnajady M.A., Eskandarloo H., Characterization and Photocatalytic Activity of Ag–Cu/TiO2 Nanoparticles Prepared by Sol–Gel Method, J Nanosci Nanotechnol, 2013, 13, 1,548-553(6).10.1166/jnn.2013.6859Search in Google Scholar
 Ubonchonlakate K., Sikong L., Saito F., Photocatalytic disinfection of P.aeruginosa bacterial Ag-doped TiO2 film, Procedia Engineering, 2012, 32, 656–662.10.1016/j.proeng.2012.01.1323Search in Google Scholar
 Subba K.V., Lavedrine B., Boule P., Influence of metallicspecies on TiO2 for the photocatalytic degradation of dyes and dye intermediates, J. Photochem. Photobiol. A: Chem. 2003, 154, 189–193.10.1016/S1010-6030(02)00299-XSearch in Google Scholar
 Yu J., Xiong J., Cheng B., Liu S., Fabrication and characterization of Ag-TiO2 multiphase nanocomposite thin films with enhanced photocatalytic activity, Appl. Catal. B:Environ., 2005, 60, 211–221.10.1016/j.apcatb.2005.03.009Search in Google Scholar
 Seery M.K., George R., Floris P., Pillai S.C., Silver doped titanium dioxide nanomaterials for enhanced visible light photocatalysis, J. Photochem. Photobiol. A: Chem., 2007, 189, 258–263.10.1016/j.jphotochem.2007.02.010Search in Google Scholar
 Kubacka A., Ferrer M., Martínez-Arias A., Fernández-García M., Ag promotion of TiO2-anatase disinfection capability: study of Escherichia coli inactivation, Appl. Catal. B: Environ., 2008, 84, 1–2, 87–93.10.1016/j.apcatb.2008.02.020Search in Google Scholar
 Ipsita H.C., Ghosh S., Naskar M.K., Aqueous-based synthesis of mesoporous TiO2 and Ag-TiO2 nanopowders for efficient photodegradation of methylene blue, Ceram. Int., 2016, 42, 2488–2496.10.1016/j.ceramint.2015.10.049Search in Google Scholar
 Xiaoyang P., Yi-Jun X., Defect-Mediated Growth of Noble-Metal (Ag, Pt, and Pd) Nanoparticles on TiO2 with Oxygen Vacancies for Photocatalytic Redox Reactions under Visible Light, J. Phys. Chem. C, 2013, 117, 17996–18005.10.1021/jp4064802Search in Google Scholar
 Xu J., Xiao X., Ren F., Wu W., Dai Z., Cai G., Zhang S., Zhou J., Mei F., Jiang C., Enhanced photocatalysis by coupling of anatase TiO2 film to triangular Ag nanoparticle island, Nanoscale Research Letters, 2012, 10.1186/1556–276X-7-239.Search in Google Scholar
 Yin S., Hasegawa H., Maeda D., Ishitsuka M., Sato T., Synthesis of visible-light-active nanosize rutile titania photocatalyst by low temperature dissolution reprecipitation process, J. Photochem. Photobiol. A: Chem., 2004, 163, 1–8.10.1016/S1010-6030(03)00289-2Search in Google Scholar
 Ashkarran A., Aghigh S., Kavianipour M., and Farahani N., Visible Light Photo-and Bioactivity of Ag/TiO2 Nanocomposite with Various Silver Contents, Current Applied Physics, 2011, 11, 1048–1055.10.1016/j.cap.2011.01.042Search in Google Scholar
 Goei R., Lim T. T., Ag-decorated TiO2 photocatalytic membrane with hierarchical architecture: photocatalytic and anti-bacterial activities, Water Res., 2014, 59, 207–218.10.1016/j.watres.2014.04.025Search in Google Scholar PubMed
 Anderson S.R., Mohammadtaheri M., Kumar D., O’Mullane A.P., Field M.R.,. Ramanathan R and Bansal V.l, Robust Nanostructured Silver and Copper Fabrics with Localized Surface Plasmon Resonance Property for Effective Visible Light Induced Reductive Catalysis, Biotechnol. Adv., 2016, 3, 6.10.1002/admi.201500632Search in Google Scholar
 Dastjerdi R., Montazer M., A review on the application of inorganic nano-structured materials in the modification of textiles: Focus on anti-microbial properties, Colloids Surf., B: Biointerfaces, 2010, 79, 5–18.10.1016/j.colsurfb.2010.03.029Search in Google Scholar PubMed
 IKaba S., Egorova E.M., In vitro studies of the toxic effects of silver nanoparticles on HeLa and U937 cells Nanotechnology, Science and Applications, 2015, 8, 19–29.10.2147/NSA.S78134Search in Google Scholar PubMed PubMed Central
 Hartemann P., Hoet P., Proykova A., Fernandes T., Baun A., De Jong W., Filser J., Hensten A., Kneuer C.,. Maillard J.-Y. Norppa H., Scheringer M., Wijnhoven S., Nanosilver: Safety, health and environmental effects and role in antimicrobial resistance, Materials Today, 2015, 18, 3.10.1016/j.mattod.2015.02.014Search in Google Scholar
 Xu H., Qu F., Xu H., Lai W., Wang Y. A., Aguilar Z.P., Wei H., Role of reactive oxygen species in the antibacterial mechanism of silver nanoparticles on Escherichia coli O157:H7, Biometals 2012, 25:45–53 10.1007/s10534-011-9482-x.Search in Google Scholar PubMed
 Yu B., Leung K.M., Guo Q., Lau W.Ming and Yang J., Synthesis of Ag-TiO2 composite nano thin film for antimicrobial application, Nanotechnology, 2011, 22, 11.10.1088/0957-4484/22/11/115603Search in Google Scholar PubMed
 Gaidau C., Petica A., Dragomir T., lovu H., and Andronescu C., Ag and Ag/TiO2 nano-dispersed systems for treatment of leathers with strong antifungal properties, J. Amer. Leather Chem. Ass, 2011, 106, 3, 102–109.Search in Google Scholar
 Christopher P., Ingram D.B. and Linic S., Enhancing Photochemical Activity of Semiconductor Nanoparticles with Optically Active Ag Nanostructures: Photochemistry Mediated by Ag Surface Plasmons, J. Phys. Chem. C, 2010, 114, 9173–9177.10.1021/jp101633uSearch in Google Scholar
 Anicai L., Petica A., Gavriliu S., Electrochemical procedure of obtaining ecologic disperse nanostructured systems with photocatalytic and antimicrobial activity”, RO.Patent no.125498/2012.Search in Google Scholar
 Petica A., Gavriliu S., Lungu M., Buruntea N., Panzaru C., Colloidal Silver Solutions with Antimicrobial Properties, Mater. Sci. Eng., B, 2008, 152, 22–27.10.1016/j.mseb.2008.06.021Search in Google Scholar
 Bitlisi B. O., Yumurtas A., Self cleaning leathers-the effect of nano TiO2, J. Soc. Leather Technol.Chem, 2008, 92, 5, 183–186.Search in Google Scholar
 Petica A., Gaidau C., Ignat M., Sendrea C., Anicai L., Doped TiO2 Nanophotocatalysts for Leather Surface Finishing with Self-Cleaning Properties, J. Coat. Technol. Res., 2015, 12, 6, 1153–1163.10.1007/s11998-015-9711-2Search in Google Scholar
 Krejcikova S., Matejova L., Koci K., Obalova L., Matej Z., Capek L., Solcova O., Preparation and characterization of Ag-doped crystalline titania for photocatalysis applications, Appl.Catal. B. Environ., 2012, 111–112, 119–125.10.1016/j.apcatb.2011.09.024Search in Google Scholar
 Arabatzis I.M., Stergiopoulos T., Bernard M.C., Labou D., Neophytides S.G., Falaras P., Silver-modified titanium dioxide thin films for efficient photodegradation of methyl orange, Applied Catalysis B: Environmental, 2003, 42, 2, 187–201.10.1016/S0926-3373(02)00233-3Search in Google Scholar
 Liu S.X., Qu Z.P., Han X.W. and Sun C.L., A mechanism for enhanced photocatalytic activity of silver-loaded titanium dioxide, Catal. Today, 2004, 93, 877–884.10.1016/j.cattod.2004.06.097Search in Google Scholar
 Dhabbe R. S., Kadam A. N., Suwarnkar M. B., Kokate M. R., Garadkar M., Enhancement in the photocatalytic activity of Ag loaded N-doped TiO2 nanocomposite under sunlight, Journal of Materials Science: Materials in Electronics, 2014, 25, 3179–3189.10.1007/s10854-014-2001-4Search in Google Scholar
 Feng N., Wang Q., Zheng A., Zhang Z., Fan J., Liu S.-B., Amoureux J.-P., and Deng F., Understanding the High Photocatalytic Activity of (B, Ag)-Codoped TiO2 under Solar-Light Irradiation with XPS, Solid-State NMR, and DFT Calculations, J. Am. Chem. Soc., 2013, 135, 1607–1616.10.1021/ja312205cSearch in Google Scholar PubMed
 Khan M. M., Ansari S.A., Amal M. I., Lee J. and Cho M.H., Highly visible light active Ag@TiO2 nanocomposites synthesized using an electrochemically active biofilm: a novel biogenic approach, Nanoscale, 2013, 5, 4427–4435.10.1039/c3nr00613aSearch in Google Scholar PubMed
 Ni M., Leung M.K., Leung D.Y., Sumathy K., A review and recent developments in photocatalytic water-splitting using TiO2 for hydrogen production, Renew. Sustain. Energ. Rev, 2007, 11,, 401–425.10.1016/j.rser.2005.01.009Search in Google Scholar
 Pelaez M., Nolan N. T., Pillai S. C., Seery M. K., Falaras P., A review on the visible light active titanium dioxide photocatalysts for environmental applications, Applied Catalysis B: Environmental, 2012, 125, 331–349.10.1016/j.apcatb.2012.05.036Search in Google Scholar
 Xu Q., Ma J., Fan Q., Yan Z., Design and Fabrication of Casein-based TiO2 Nanocomposite for Self-cleaning Leather Finishes, In: Proceeding of XXXIII IULTCS Congress November (24th – 27th, 2015 Novo Hamburgo/Brazil), 026.Search in Google Scholar
 Iordache D., Kientz E., Fennen J., Leather topcoats with antisoiling and non-squeak properties, World Leather, 2012, 1, 13–16.Search in Google Scholar
 Schmid H., Antimicrobial functionalization of surfaces using nanosilver technology-a safe, effective and cost-effective means of reducing hospital infections, Nano Magazine, 2014, 28, 2, 17–20.Search in Google Scholar
 Yang W., Wang X., Gong Y., Li H., Chen W. and Gaidau C., Preparation of Antibacterial Sheepskin With Silver Nanoparticles, Potential for Use as a Mattress for Pressure Ulcer Prevention, J. Amer. Leather Chem. Ass., 2012, 107, 85–92.Search in Google Scholar
 Gaidau C., Petica A., Micutz M., Danciu M., Vladkova T., Progresses in Treatment of Collagen and Keratin Based Materials with Silver Nanoparticles, Central European Journal of Chemistry, 2013, 11, 901–911.10.2478/s11532-013-0224-5Search in Google Scholar
 Thomas J., Jacobson G.A., Narkowicz C.K., Peterson G.M., Burnet H., Sharpe C., Toenail onychomycosis: an important global disease burden, Journal of Clinical Pharmacy and Therapeutics, 2010, 35, 497–519.10.1111/j.1365-2710.2009.01107.xSearch in Google Scholar PubMed
 Vazquez-Muñoz R., Avalos-Borja M. and Castro-Longoria E., Ultrastructural Analysis of Candida albicans When Exposed to Silver Nanoparticles, .PLoS One. 2014; 9(10): e108876.10.1371/journal.pone.0108876Search in Google Scholar PubMed PubMed Central
 Huanjun Zh., and Guohua Ch., Potent Antibacterial Activities of Ag/TiO2 Nanocomposite Powders Synthesized by a One-Pot Sol-Gel Method, Environmental Science & Technology, 2009, 43, 2905–2910.10.1021/es803450fSearch in Google Scholar PubMed
 Wu T.S., Wang K.-X., Li G.-D., Sun S.-Y., Sun J. and Chen J.-S., Montmorillonite-Supported Ag/TiO2 Nanoparticles: An Efficient Visible-Light Bacteria Photodegradation Material, ACS Appl. Mater. Interfaces, 2010, 2, 544–550.10.1021/am900743dSearch in Google Scholar PubMed
 Yali Y., Jianqiang D., Jinsheng X., Jian D., Jianbo G., TiO2 Nanoparticles Co-Doped with Silver and Nitrogen for Antibacterial Application, J Nanosci Nanotechnol, 2010, 10, 8, 4868–4874(7).10.1166/jnn.2010.2225Search in Google Scholar PubMed
 Quiñones-Jurado Z. V., Waldo-Mendoza M. Á., Bandin H. M. A., Villabona-Lea E. G., Cervantes-González E., Pérez E., Silver Nanoparticles Supported on TiO2 and Their Antibacterial Properties: Effect of Surface Confinement and Nonexistence of Plasmon Resonance, Materials Sciences and Applications, 2014, 5, 895–903.10.4236/msa.2014.512091Search in Google Scholar
© 2016 Carmen Gaidau et al.
This work is licensed under the Creative Commons Attribution-NonCommercial-NoDerivatives 3.0 License.